text: The Krupp–Renn process is a direct reduction process that uses a long tubular furnace similar to those found in cement production. The most recent units constructed have a diameter of approximately 4.5 meters and a length of 110 meters. The residence time of the product is influenced by the slope and speed of rotation of the rotary kiln, which is inclined at an angle of roughly 2.5 percent.
  Prior to usage, the iron ore is crushed to less than 6 mm in particle size. The iron ore is introduced into the furnace upstream and mixed with a small amount of fuel, typically hard coal. After 6 to 8 hours, it exits the furnace as pre-reduced iron ore at 1,000 °C. The amount of iron recovered ranges from 94% to 97.5% of the initial iron in the ore.
  A burner located at the lower end of the furnace provides heat, transforming it into a counter-current reactor. The fuel comprises finely pulverized coal, which, upon high-temperature combustion, generates reducing gas primarily consisting of CO. Once the furnace reaches an optimal temperature, the ore-coal mixture can serve as the primary fuel source.
  The fumes exiting the furnace's upper end attain temperatures ranging from 850 to 900 °C and are subsequently cooled and purged of dust by water injection before discharge through the chimney.
  The process is efficient in producing ferronickel due to the proximity of its constituent elements. At 800 °C, carbon easily reduces iron and nickel oxides, while the gangue's other oxides are not significantly reduced. Specifically, iron(II) oxide (or wustite), which is the stable iron oxide at 800 °C, has a reducibility similar to that of nickel(II) oxide, making it impossible to reduce one without reducing the other.